Download presentation

Presentation is loading. Please wait.

Published byEmilee Cayson Modified about 1 year ago

1
Virtual Glass Course — 1 Modeling & Simulation of Glass Structure VCG Lecture 21 John Kieffer Department of Materials Science and Engineering University of Michigan

2
Virtual Glass Course — 2 Overview … Historical perspective Simulation methodologies Theoretical background Monte Carlo simulation Molecular dynamics simulation Reverse Monte Carlo Force fields Information retrieval Statistical mechanical formalisms Structural analyses Dynamics Application examples

3
Virtual Glass Course — 3 Force Fields Types of interactions between two molecules Electrostatic interactions Between charges (if ions) and between permanent dipoles, quadrupoles and higher multipole moments –May be represented through partial charges Embedding terms (metals) Induction interactions Between, for example, a permanent dipole and an induced dipole Dispersion interactions Long-range attraction that has its origin in fluctuations of the charge distribution Valence (overlap) interactions Covalent bonds Repulsive interaction at short range which arises from exclusion principle Residual valence interactions Specific chemical forces giving rise to association and complex formation - e.g., hydrogen bonding Types of interactions within a molecule Bond stretch, bond-angle bending, torsional potential r

4
Virtual Glass Course — 4 Force Fields Non-bonded interactions are typically long-range and involve a large number of particles. Yet, contributions to the total energy and forces are considered as pair- wise additive ++ ++ -- Non-bonded (van der Waals) Non-bonded (electrostatic) Johannes Diderik Van der Waals

5
Virtual Glass Course — 5 Metals Example: Morse force field Approximate physical behavior Computationally efficient

6
Virtual Glass Course — 6 Van der Waals interactions The most popular model of the van der Waals non-bonded interactions between atoms is the Lennard-Jones potential. Sir John Edward Lennard-Jones U(r) r = r ij minimum at r=1.122 typical cutoff at 2.5 Collision diameter

7
Virtual Glass Course — 7 Metals Embedded atom method

8
Virtual Glass Course — 8 Metals Embedded atom method

9
Virtual Glass Course — 9 Embedded atom method E c = cohesive energy B = bulk modulus = atomic volume Other factors are model parameters that are determined based on lattice parameter, bulk modulus, shear modulus, cohesive energy, vacancy formation energy, and average electron density

10
Virtual Glass Course — 10 Formation of dislocations in metals V. Bulatov, LLNL

11
Virtual Glass Course — 11 Simulation of Laser Ablation on Metal Surface G.H. Gilmer, LLNL 3·10 6 atoms x 140 ps

12
Virtual Glass Course — 12 Embedded atom method Simple closed form Computationally efficient Based on density functional theory concept Accurate for highly symmetric structures (FCC, BCC) Accurate for spherical electron orbitals Increasingly inaccurate for complex atomic electron configurations and low-symmetry structures

13
Virtual Glass Course — 13 Range of interactions Short-range interactions: 1/2·N·N C force calculations Long-range interactions: 1/2·N·(N-1) force calculations

14
Virtual Glass Course — 14 Ionic Materials Coulomb interactions are fundamental to atomistic systems Coulomb interactions have long-range effects

15
Virtual Glass Course — 15 Ionic Materials Degree of charge localization can vary Charge polarization effects can be accounted for analytically

16
Virtual Glass Course — 16 Ionic Materials Repulsion due to electron orbital overlap Repulsion due to interactions between nuclei … handled by empirical function

17
Virtual Glass Course — 17 The trouble with Coulomb interactions

18
Virtual Glass Course — 18 The trouble with Coulomb interactions Conditionally convergent … I.e., depends on how one adds it up …

19
Virtual Glass Course — 19 Long-range interactions: Ewald summation method Total potential energy of one ion at the reference point. Summation decomposed into two parts, one to be evaluated in real space, the other in reciprocal space. …

20
Virtual Glass Course — 20 Reciprocal space

21
Virtual Glass Course — 21 Reciprocal space

22
Virtual Glass Course — 22 Reciprocal space

23
Virtual Glass Course — 23 Reciprocal space

24
Virtual Glass Course — 24 Reciprocal space

25
Virtual Glass Course — 25 Reciprocal space At r = 0: Self-energy correction

26
Virtual Glass Course — 26 Real space

27
Virtual Glass Course — 27 Convergence in real and reciprocal space

28
Virtual Glass Course — 28 Molecular Simulation Massively parallel molecular dynamics Spatial domain decomposition - large systems Replicated data - long simulation times

29
Virtual Glass Course — 29 Spatial Decomposition and Ewald Sum 11 2 > 1 Requires larger G

30
Virtual Glass Course — 30 Particle-Mesh Ewald Method f [u] interpolation function

31
Virtual Glass Course — 31 Example: fracture in brittle materials

32
Virtual Glass Course — 32 Overview … Historical perspective Simulation methodologies Theoretical background Monte Carlo simulation Molecular dynamics simulation Reverse Monte Carlo Force fields Information retrieval Statistical mechanical formalisms Structural analyses Dynamics Application examples

33
Virtual Glass Course — 33 Ionic materials Fundamentally correct Accurate for strongly ionic compounds, including many ceramics and salts … Long-range interactions cause computational expense Increasingly inaccurate when partially covalent interactions and charge transfer occurs

34
Virtual Glass Course — 34 Questions?

35
Virtual Glass Course — 35 “Universal” force fields Goal is to develop force field that can be to describe intra- and inter-molecular interactions for arbitrary molecules UFF (Universal force field) A. K. Rappe, C. J. Casewit, K. S. Colwell, W. A. Goddard and W. M. Skiff, "UFF, a Full Periodic-Table Force-Field for Molecular Mechanics and Molecular-Dynamics Simulations," J. Am. Chem. Soc, 114, (1992) Used for many nanoscale carbon structures (buckyballs, nanotubes) COMPASS (Condensed-phase Optimized Molecular Potentials for Atomistic Simulation Studies) Sun, H; Rigby, D. "Polysiloxanes: Ab Initio Force Field And Structural, Conformational And Thermophysical Properties", Spectrochimica Acta (A),1997,53, 130, and subsequent references AMBER (Assisted Model Building with Energy Refinement) Both a force field and a simulation package for biomolecular simulations

36
Virtual Glass Course — 36 “Universal” force fields CHARMM (Chemistry at HARvard Macromolecular Mechanics ) Both a force field and a simulation package for biomolecular simulations B. R. Brooks, R. E. Bruccoleri, B. D. Olafson, D. J. States, S. Swaminathan, and M. Karplus, “A Program for Macromolecular Energy, Minimization, and Dynamics Calculations, J. Comp. Chem. 4 (1983) (1983) Others GROMOS (http://www.igc.ethz.ch/gromos)http://www.igc.ethz.ch/gromos Jorgensen’s Optimized Potential for Liquid Simulation (OPLS) (http://zarbi.chem.yale.edu)http://zarbi.chem.yale.edu DREIDING (Mayo, S. L., Olafson, B. D. & Goddard, W. A. Dreiding - a Generic Force- Field for Molecular Simulations. Journal of Physical Chemistry 94 (1990) ) Specific systems Alkanes and related systems –SKS: B. Smit, S. Karaborni, and J.I. Siepmann, `Computer simulation of vapor- liquid phase equilibria of n-alkanes', J. Chem. Phys. 102, (1995); `Erratum', 109, 352 (1998) –TraPPE: Siepmann group (http://siepmann6.chem.umn.edu)

37
Virtual Glass Course — 37 Latest trends: Charge transfer Charge localization depends on environment Chemical nature of surrounding atoms Local structure Electronegativity Atomic hardness IP = first ionization potential; EA = electron affinity

38
Virtual Glass Course — 38 Charge transfer Energy of an isolated atom: Energy of an N atoms:

39
Virtual Glass Course — 39 Charge transfer Spherically symmetric Slater-type orbitals are assumed for (r)

40
Virtual Glass Course — 40 Charge transfer Chemical potential of electrons associated with atom i: Equilibrium requires 1 = 2 = 3 = … = N, which yields N–1 equations. In addition, charge neutrality requires that

41
Virtual Glass Course — 41 Charge transfer Solving the system of equations yields the equilibrium charges Equilibrium charges depend on the chemical nature of species and on the geometry of the configuration, by virtue of the fact that

42
Virtual Glass Course — 42 torque covalent attractive Coulomb repulsive charge transfer function total Covalently bonded materials Directional character of bonds Covalent bonding term (empirical), e.g.,

43
Virtual Glass Course — 43 Reactive force fields … Charge redistribution Flexible coordination L. P. Huang and J. Kieffer, J. Chem. Phys. 118, 1487 (2003)

44
Virtual Glass Course — 44 Force field parameterization Reproduce known structures (static properties) density at ambient pressure equation of state (density vs. pressure) mechanical properties (elastic moduli, strength, etc.) Reproduce dynamic properties melting temperatures vibrational spectra Compare with results from ab initio calculations bonding energies Interatomic forces

45
Virtual Glass Course — 45 Crystalline silica polymorphs – one parameterization 16 GPa (C222 1 ) a’ = 6.7 Å b’ = 5.7 Å c’ = 6.1 Å c’ a’ 20 GPa (P ) a = 4.2 Å b = 4.2 Å c = 6.0 Å 0 GPa (P ) a = 4.9 Å b = 4.9 Å c = 5.4 Å 25 GPa (P42/mnm) a = 4.2 Å b = 4.2 Å c = 2.8 Å 14 GPa (P ) 40 GPa (Pnnm) a = 3.7 Å b = 4.5 Å c = 2.8 Å X-I phase -cristobalite stishovitepost-stishovite -quartz at 0 GPa High-P quartz at 25 GPa Ideal high-P quartz with bcc anion sub-lattice Huang, Durandurdu and Kieffer, Nature Materials (in press)

46
Virtual Glass Course — 46 Parameter Optimization: Crystal Structures 291K, NVT, 64 molecules J. Chem. Soc. Dalton Trans. 1994, (Hexyl-POSS)

47
Virtual Glass Course — 47 Parameter Optimization: IR Spectrum J. Chem. Soc. Dalton Trans. 1994,

48
Virtual Glass Course — 48 Parameter Optimization: Fitting to Electronic Structure Calculations High Intermediate Low POSS-NaCl Potential Surface

49
Virtual Glass Course — 49 Fitting Results MullikenpointshellEEM Si O H ~0.01 ( E)

50
Virtual Glass Course — 50 Charge Equilibration Method

51
Virtual Glass Course — 51 Questions?

52
Virtual Glass Course — 52 QM Methods Doing a QM simulation or calculation means including the electrons explicitly. With QM methods, we can calculate properties that depend upon the electronic distribution, and to study processes like chemical reactions in which bonds are formed and broken. The explicit consideration of electrons distinguishes QM models and methods from classical force field models and methods.

53
Virtual Glass Course — 53 Different QM Methods Several approaches exist. The two main ones are: Molecular orbital theory Came from chemistry, since primarily developed for individual molecules, gases and now liquids. Two “flavors” –Ab initio: all electrons included (considered exact) –Semi-empirical: only valence electrons included Density functional theory Came from physics and materials science community, since originally conceived for solids. All electrons included via electronic density (considered exact).

54
Virtual Glass Course — 54 Fundamentals The operator that returns the system energy is called the Hamiltonian operator H. H = E Time-independent Schrodinger Equation Kinetic energy of electrons Kinetic energy of nuclei Potential energy of electrons & nuclei Potential energy of electrons Potential energy of nuclei Eigenvalue equation for system energy

55
Virtual Glass Course — 55 Born-Oppenheimer Approximation Neutrons & protons are >1800 times more massive than electrons, and therefore move much more slowly. Thus, electronic “relaxation” is for all practical purposes instantaneous with respect to nuclear motion. We can decouple the motion, and consider the electron-electron interactions independently of the nuclear interactions. This is the Born- Oppenheimer approximation. For nearly all situations relevant to soft matter, this assumption is entirely justified. (H el +V n ) el (q i ;q k ) = E el el (q i ;q k ) The Electronic Schrodinger Equation Need to simplify!

56
Virtual Glass Course — 56 QM Methods Goal of all QM methods in use today: Solve the electronic Schrodinger equation for the ground state energy of a system and the wavefunction that describes the positions of all the electrons. The energy is calculated for a given trial wavefunction, and the “best” wavefunction is found as that wavefunction that minimizes the energy.

57
Virtual Glass Course — 57 QM Methods Solving SE is not so easy! Anything containing more than two elementary particles (i.e. one e- and one nucleon) can’t be solved exactly: the “many-body problem”. Even after invoking Born-Oppenheimer, still can’t solve exactly for anything containing more than two electrons. So -- all QM methods used today are APPROXIMATE after all, even if considered “exact”! That is, they provide approximate solutions to the Schrodinger equation. Some are more approximate than others.

58
Virtual Glass Course — 58 Molecular Orbital Theory MOT is expressed in terms of molecular wave functions called molecular orbitals. Most popular implementation: write molecular orbital as a linear combination of atomic orbitals (LCAO): Many different ways of writing “basis set”, which leads to many different methods and implementations of MOT. Eq in Leach K = # atomic orbitals

59
Virtual Glass Course — 59 Molecular Orbital Theory Dozens of approaches for writing basis sets (e.g. in terms of Gaussian wavefunctions, or as linear combos of Gaussians). Different implementations retain different numbers of terms. Semi-empirical MOT methods consider only valence electrons. Some methods include electron exchange. Some methods include electron correlation.

60
Virtual Glass Course — 60 Density Functional Theory A different approach for solving Schrodinger’s equation for the ground state energies of matter. Based on theory of Hohenberg and Kohn (1964) which states that it is not necessary to consider the motion of each individual electron in the system. Instead, it suffices to know the average number of electrons at any one point in space. The HK theorem enables us to write E el as a functional of the electron density To perform a DFT calculation, one optimizes the energy with respect to the electron probability density, rather than with respect to the electronic wave function. For a given density, the lowest energy is the best one.

61
Virtual Glass Course — 61 Density Functional Theory In the commonly used Kohn-Sham implementation, the density is written in terms of one-electron molecular orbitals called “Kohn-Sham orbitals”. This allows the energy to be optimized by solving a set of one-electron Schrodinger equations (the KS equations), but with electron correlation included. This is a key advantage of the DFT method - it’s easier to include electron correlation. Different choices of basis sets, how many terms to use, of what type, contribute to difficulty of calculation. More than a few hundred light atoms is still too time-consuming, even on big computers. For molecules or systems with large numbers of electrons, pseudopotentials are used to represent the wavefunctions of valence electrons, and the core is treated in a simplified way.

62
Virtual Glass Course — 62 Applications of ab initio computations using DMol 3

63
Virtual Glass Course — 63 Electronic band structure of POSS cubes functionalized with n benzene molecules (n = 0-8) … Energy (eV)

64
Virtual Glass Course — 64 Electronic band structure of POSS cubes functionalized with acene molecules (benzene, naphtalene, anthracene, tetracene, and pentacene) Energy (eV) Pure poss

65
Virtual Glass Course — 65 Electron densities of acene-functionalized POSS HOMOLUMO Molecule Band Gap (eV) Pure Acene (eV) P-POSS T-POSS A-POSS N-POSS B-POSS POSS8.4-

66
Virtual Glass Course — 66 Electron densities of silica nanotubes HOMOLUMO

67
Virtual Glass Course — 67 Classical vs. ab initio methods No electronic properties Phenomenological potential energy surface (typically 2- body contributions) Difficult to describe bond breaking/formation Can do up to a billion particles Electronic details included Potential energy surface calculated directly from Schrodinger equation (many body terms included automatically) Describes bond breaking/formation Limited to several hundred atoms with significant dynamics Classical ab initio

68
Virtual Glass Course — 68 Questions? Editor’s Note: Lecture 21 ended here – 4/2/07

69
Virtual Glass Course — 69 Overview … Historical perspective Simulation methodologies Theoretical background Monte Carlo simulation Molecular dynamics simulation Reverse Monte Carlo Force fields Information retrieval Statistical mechanical formalisms Structural analyses Dynamics Application examples

70
Virtual Glass Course — 70 Simulation Observables: Thermodynamics In a classical, many body system, the temperature is defined from the equipartition theorem in terms of the average kinetic energy per degree of freedom: In a simulation, we use this equation as an operational definition of T. Thus the lower the temperature, the lower the kinetic energy, and the slower the average velocity.

71
Virtual Glass Course — 71 time steps Simulation Observables: Thermodynamics Thermodynamic quantities Calculate T, , p, E etc. depending on ensemble NVE N c = # of constraints (e.g. linear momentum) 3N - N c = # of degrees of freedom

72
Virtual Glass Course — 72 Pressure Simulation Observables: Thermodynamics NVE time steps P is obtained from the virial thm of Clausius. Virial = exp. value of the sum of the products of the particle coords and the forces acting on them. W= x i f xi =-3Nk B T

73
Virtual Glass Course — 73 Measuring quantities in molecular simulations Suppose we wish to measure in an experiment the value of a property, A, of a system such as pressure or density or heat capacity. The property A will depend on the positions and momenta of the N atoms or molecules that comprise the system. The instantaneous value of A is: A(p N (t),r N (t)) = A(p 1x,p 1y,p 1z, …, x 1,y 1,z 1,…t). Over time, A fluctuates due to interactions between the atoms.

74
Virtual Glass Course — 74 Measuring quantities in molecular simulations In any experiment, the value that we measure is an average of A over the time of the measurement (a time average). As the time, t, of the measurement increases to infinity, the “true” average value of A is attained: Note that strictly speaking this is true only for ergodic systems in equilibrium.

75
Virtual Glass Course — 75 Measuring quantities in molecular simulations To calculate properties in a molecular simulation, we average a property A over successive configurations in the trajectory generated by the equations of motion. The larger n steps is, the more accurate the estimate of the true time-averaged value of A.

76
Virtual Glass Course — 76 Ensemble averages In statistical mechanics we learn that experiments and simulations may be performed in different ensembles. An ensemble is a collection of individual systems that can be studied en masse to yield macroscopic properties of the entire collection. Every equilibrium configuration we generate via MD represents a unique microstate of the ensemble.

77
Virtual Glass Course — 77 Ensemble averages There are many different thermodynamic ensembles, each of which is characterized by thermodynamic variables that are fixed in the simulation. NVE - microcanonical NVT - canonical NPT - isobaric-isothermal VT - Gibbs N = number of particles, V = volume, E = total energy, T = temperature, P = pressure, = chemical potential The simplest MD simulation has constant N, V and E. The NVE ensemble is the microcanonical ensemble; all states are equally likely. In NVE MD, solve F=ma for an isolated system, one for which no exchange of energy or particles with the outside.

78
Virtual Glass Course — 78 Molecular Dynamics Simulation: NVT Velocity Rescaling Recall KE = mv 2 /2 = 3Nk B T/2 in an unconstrained system. Simple way to alter T: rescale velocities every time step by a factor (t): If temperature at time t is T(t) and v is multiplied by then the temperature change is

79
Virtual Glass Course — 79 Molecular Dynamics Simulation: NVT Velocity Rescaling This method does not generate configurations in the canonical ensemble. Why? Because system is not coupled to an external reservoir, or heat bath. Thus not a good method for controlling temperature, since it’s unknown how rescaling affects properties of the system. Instead, use a “proper” thermostat. Using a weakly coupled thermostat can help eliminate drift in total energy due to algorithm inaccuracies and round-off error. Several types of thermostats; choose wisely depending on your problem!

80
Virtual Glass Course — 80 Molecular Dynamics Simulation: NVT Stochastic collision method: Andersen thermostat Occasionally replace a randomly chosen particle’s velocity with a velocity chosen randomly from a Maxwell-Boltzmann distribution at the desired T. This replacement represents stochastic collisions with the heat bath. Equivalent to the system being in contact with a heat bath that randomly emits thermal particles that collide with the atoms in the system and change their velocity.

81
Virtual Glass Course — 81 Molecular Dynamics Simulation: NVT Extended system method: Nose’-Hoover thermostat Introduced by Nose’ and developed by Hoover in Considers the thermostat to be part of the system (hence ‘extended system’). Based on extended Lagrangian approach in which an additional dynamical variable or degree of freedom s, representing the reservoir, imposes constraint of constant T. reservoir physical system extended system

82
Virtual Glass Course — 82 Molecular Dynamics Simulation: NVT Extended system method: Nose’-Hoover thermostat Reservoir has potential energy U res and kinetic energy K res. f = # of dof in physical system, and T is the desired temperature. Q has dimensions energy x (time) 2, and is considered the fictitious “mass” of the additional degree of freedom. The magnitude of Q controls the coupling between the physical system and the reservoir, and thus influences the temperature fluctuations. reservoir physical system U res = (f+1)k B T ln s K res = (Q/2)(ds/dt) 2

83
Virtual Glass Course — 83 Molecular Dynamics Simulation: NVT Extended system method: Nose’-Hoover thermostat Q controls the energy flow between system and reservoir. If Q is large, the energy flow is slow; the limit of infinite Q corresponds to NVE MD since there is then no exchange of energy between system and reservoir. If Q is small, then the energy oscillates unphysically, causing equilibration problems. Nose’ suggested Q = Cfk B T, where C can be obtained by performing trial simulations for a series of test systems and observing how well the system maintains that desired T. Upshot: equations of motion are modified and t is multiplied by Q. Read in Frenkel and Smit for details if interested.

84
Virtual Glass Course — 84 Molecular Dynamics Simulation: NVT Extended system method: Nose’-Hoover thermostat Best and most used thermostat today for NVT simulations. Ensures that average total KE per particle is that of the equilibrium isothermal ensemble. Reproduces canonical ensemble in every respect (provided only the total energy of the extended system is conserved.) If momentum also conserved, NH still works only if COM fixed. Otherwise, must use the method of “NH chains”. More complicated than other methods, but can be used with velocity Verlet and predictor-corrector methods. Dynamics NOT independent of Q, but better than Andersen.

85
Virtual Glass Course — 85 Molecular Dynamics Simulation: NPT Just as one might like to specify T in an MD simulation, one might also like to maintain the system at a fixed pressure P. Simulations in the isobaric-isothermal NPT ensemble are the most similar to experimental conditions. Certain phenomena may be more easily achieved under conditions of constant pressure, like certain phase transformations.

86
Virtual Glass Course — 86 Molecular Dynamics Simulation: NPT Two types: Andersen Barostat Allows box size to fluctuate but not change shape. Appropriate for liquids, which do not support shear stress. Change volume by rescaling positions: r = r+ r Rahman-Parinello Barostat Allows box size and shape to change. Use only for solids. Necessary for simulating phase transformations. Read in Frenkel and Smit for details if interested.

87
Virtual Glass Course — 87 Revisit the equations of motion … Recall Lagrangian

88
Virtual Glass Course — 88 Flexible simulation boxes Mechanical deformation Structural transitions

89
Virtual Glass Course — 89 Raman-Parinello algorithm a b c Basis vectors are dynamical variables:

90
Virtual Glass Course — 90 Raman-Parinello algorithm Raman-Parinello Nosé-Hoover algorithm

91
Virtual Glass Course — 91

92
Virtual Glass Course — 92 Thermodynamic Response Functions: Heat Capacity NVE: Perform simulations at many different E for the same N & V, and measure T. Calculate C v from derivative of E(T) (numerically or fitting polynomial and then differentiating). NVT: (1) Fix N and V, perform simulations at different T and measure E. Then calculate C v from derivative of E(T). (2) Calculate C v from fluctuations in energy. Simulation Observables: Thermodynamics - 2 On the fly At the end (less error?)

93
Virtual Glass Course — 93 Thermodynamic Response Functions: Adiabatic Compressibility NVE: (1) Fix N and E, perform simulations at different V and measure P. Calculate S from derivative of V(P). (2) Calculate S from fluctuations in pressure. NVT: Calculate S from fluctuations in pressure. Simulation Observables: Thermodynamics

94
Virtual Glass Course — 94 Thermodynamic Response Functions: Isothermal Compressibility NVT: Fix N and T, perform simulations at different V and measure P. Calculate T from derivative of V(P). NPT: Fix N and T, perform simulations at different P and measure V. Calculate T from derivative of V(P). NPT: Calculate T from fluctuations in volume. VT: Calculate T from fluctuations in N. Simulation Observables: Thermodynamics

95
Virtual Glass Course — 95 Questions?

96
Virtual Glass Course — 96 Molecular Dynamics Simulation: NPT A system maintains constant P by changing its volume, and thus to perform an NPT simulation we must allow our simulation cell to fluctuate in size. The amount of volume fluctuation is related to the isothermal compressibility An easily compressible material has a larger value of , so larger V fluctuations occur for a given change in P than in a more incompressible material.

97
Virtual Glass Course — 97 Molecular Dynamics Simulation: NPT For an ideal gas, which is very compressible, = 1 atm -1. For a simulation box 2 nm on a side (volume 8 nm 3 ) at 300K, the rms change in V is roughly 18 nm 3, which is larger than the initial size of the box. For water, which is relatively incompressible, = 44 x atm -1, and the volume fluctuation is roughly 1/10 nm 3, which corresponds to roughly 0.46 nm in one direction. These bounds give a rough idea of how we should pick the size of our simulation cell when V constant - larger than any fluctuation.

Similar presentations

© 2016 SlidePlayer.com Inc.

All rights reserved.

Ads by Google